# M n = (DP)m = (25,000)( g/mol) = 2.60! 10 6 g/mol

Save this PDF as:

Size: px
Start display at page:

Download "M n = (DP)m = (25,000)(104.14 g/mol) = 2.60! 10 6 g/mol"

## Transcription

1 14.4 (a) Compute the repeat unit molecular weight of polystyrene. (b) Compute the number-average molecular weight for a polystyrene for which the degree of polymerization is 25,000. (a) The repeat unit molecular weight of polystyrene is called for in this portion of the problem. For polystyrene, from Table 14.3, each repeat unit has eight carbons and eight hydrogens. Thus, m = 8(A C ) + 8(A H ) = (8)(12.01 g/mol) + (8)(1.008 g/mol) = g/mol (b) We are now asked to compute the number-average molecular weight. Since the degree of polymerization is 25,000, using Equation 14.6 M n = (DP)m = (25,000)( g/mol) = 2.60! 10 6 g/mol

2 14.5 Below, molecular weight data for a polypropylene material are tabulated. Compute (a) the numberaverage molecular weight, (b) the weight-average molecular weight, and (c) the degree of polymerization. Molecular Weight Range (g/mol) x i w i 8,000 16, ,000 24, ,000 32, ,000 40, ,000 48, ,000 56, (a) From the tabulated data, we are asked to compute M n, the number-average molecular weight. This is carried out below. Molecular wt Range Mean M i x i x i M i 8,000-16,000 12, ,000-24,000 20, ,000-32,000 28, ,000-40,000 36, ,080 40,000-48,000 44, ,000-56,000 52, M n =! x i M i = 33, 040 g/mol (b) From the tabulated data, we are asked to compute M w, the weight-average molecular weight. Molecular wt. Range Mean M i w i w i M i 8,000-16,000 12, ,000-24,000 20, ,000-32,000 28, ,000-40,000 36, ,800

3 40,000-48,000 44, ,880 48,000-56,000 52, M w =! w i M i = 36,240 g/mol (c) Now we are asked to compute the degree of polymerization, which is possible using Equation For polypropylene, the repeat unit molecular weight is just m = 3(A C ) + 6(A H ) = (3)(12.01 g/mol) + (6)(1.008 g/mol) = g/mol And DP = M n m 33,040 g/mol = = g/mol

4 14.8 High-density polyethylene may be chlorinated by inducing the random substitution of chlorine atoms for hydrogen. (a) Determine the concentration of Cl (in wt%) that must be added if this substitution occurs for 5% of all the original hydrogen atoms. (b) In what ways does this chlorinated polyethylene differ from poly(vinyl chloride)? (a) For chlorinated polyethylene, we are asked to determine the weight percent of chlorine added for 5% Cl substitution of all original hydrogen atoms. Consider 50 carbon atoms; there are 100 possible side-bonding sites. Ninety-five are occupied by hydrogen and five are occupied by Cl. Thus, the mass of these 50 carbon atoms, m C, is just m C = 50(A C ) = (50)(12.01 g/mol) = g Likewise, for hydrogen and chlorine, m H = 95(A H ) = (95)(1.008 g/mol) = g m Cl = 5(A Cl ) = (5)(35.45 g/mol) = g Thus, the concentration of chlorine, C Cl, is determined using a modified form of Equation 4.3 as C Cl = m Cl m C + m H + m Cl x 100 = g g g g! 100 = 20.3 wt% (b) Chlorinated polyethylene differs from poly(vinyl chloride), in that, for PVC, (1) 25% of the side-bonding sites are substituted with Cl, and (2) the substitution is probably much less random.

5 14.13 Make comparisons of thermoplastic and thermosetting polymers (a) on the basis of mechanical characteristics upon heating, and (b) according to possible molecular structures. (a) Thermoplastic polymers soften when heated and harden when cooled, whereas thermosetting polymers, harden upon heating, while further heating will not lead to softening. (b) Thermoplastic polymers have linear and branched structures, while for thermosetting polymers, the structures will normally be network or crosslinked.

6 14.14 (a) Is it possible to grind up and reuse phenol-formaldehyde? Why or why not? (b) Is it possible to grind up and reuse polypropylene? Why or why not? (a) It is not possible to grind up and reuse phenol-formaldehyde because it is a network thermoset polymer and, therefore, is not amenable to remolding. (b) Yes, it is possible to grind up and reuse polypropylene since it is a thermoplastic polymer, will soften when reheated, and, thus, may be remolded.

7 14.22 Explain briefly why the tendency of a polymer to crystallize decreases with increasing molecular weight. The tendency of a polymer to crystallize decreases with increasing molecular weight because as the chains become longer it is more difficult for all regions along adjacent chains to align so as to produce the ordered atomic array.

8 15.2 Compute the elastic moduli for the following polymers, whose stress-strain behaviors may be observed in the Tensile Tests module of Virtual Materials Science and Engineering (VMSE): (a) highdensity polyethylene, (b) nylon, and (c) phenol-formaldehyde (bakelite). How do these values compare with those presented in Table 15.1 for the same polymers? The elastic modulus is the slope in the linear elastic region (Equation 6.10) as E =! "! # = " 2 \$ " 1 # 2 \$ # 1 Since all the stress-strain curves pass through the origin, we make take σ 1 = 0 and ε 1 = 0. Determinations of σ 2 and ε 2 are possible by moving the cursor to some arbitrary point in the linear region of the curve and then reading corresponding values in the Stress and Strain windows that are located below the plot. (a) For high-density polyethylene, we selected σ 2 = 6.0 MPa with its corresponding ε 2 = Therefore, E =! 2 "! 1 # 2 " # 1 = 6.0 MPa " 0 MPa " 0 = 395 MPa = GPa The elastic modulus (average) for high-density polyethylene given in Table 15.1 is 1.08 GPa, which is significantly higher than this value. (b) For nylon, we selected σ 2 = 24.3 MPa with its corresponding ε 2 = Therefore, E =! 2 "! 1 # 2 " # 1 = 24.3 MPa " 0 MPa " 0 = 2860 MPa = 2.86 GPa The elastic modulus range for nylon 6,6 given in Table 15.1 is 1.58 GPa to 3.80 GPa; therefore, the value for the VMSE nylon lies within this range.

9 (c) For phenol-formaldehyde (bakelite), we selected σ 2 = 33.0 MPa with its corresponding ε 2 = Therefore, E =! 2 "! 1 # 2 " # 1 = 33.0 MPa " 0 MPa " 0 = 4850 MPa = 4.85 GPa The elastic modulus range for the phenol-formaldehyde given in Table 15.1 is 2.76 GPa to 4.83 GPa; therefore, this value for the VMSE phenol-formaldehyde lies just above the maximum value for this range.

10 15.3 For the nylon polymer, whose stress strain behavior may be observed in the Tensile Tests module of Virtual Materials Science and Engineering (VMSE), determine the following: (a) the yield strength, and (b) the approximate ductility, in percent elongation. How do these values compare with those for the nylon material presented in Table 15.1? (a) The yield strength corresponds to the first maximum (just beyond the initial linear-elastic region) of the stress-strain curve. This reading in the stress window located below the plot as the curser point is dragged along the stress-strain curve is 84 MPa. (b) The approximate percent elongation corresponds to the strain at fracture multiplied by 100 (i.e., 44.5%) minus the maximum elastic strain (i.e., value of strain at which the linearity of the curve ends multiplied by 100 in this case about 4%); this gives a value of about 40%EL. For nylon 6,6, the range of values of yield strength presented in Table 15.1 is 44.8 MPa to 82.8 MPa; therefore, the value for the VMSE nylon lies slightly above the upper value. The ductility range for nylon 6,6 is 15%EL to 300%EL; therefore, our value (40%EL) lies within this range.

11 15.8 On the basis of the curves in Figure 15.5, sketch schematic strain time plots for the following polystyrene materials at the specified temperatures: (a) Amorphous at 120 C (b) Crosslinked at 150 C (c) Crystalline at 230 C (d) Crosslinked at 50 C (a) Amorphous polystyrene at 120 C behaves a rubbery material (Figure 15.8, curve C); therefore, the strain-time behavior would be as Figure 15.5c. (b) Crosslinked polystyrene at 150 C behaves as a viscoelastic material (Figure 15.8, curve B); therefore, the strain-time behavior will be as Figure 15.5c. (c) Crystalline polystyrene at 230 C behaves as a viscous liquid (Figure 15.8, curve A); therefore, the strain-time behavior will be as Figure 15.5d. (d) Crosslinked polystyrene at 50 C behaves in a glassy manner (Figure 15.8, curve B); therefore, the strain-time behavior will be as Figure 15.5b.

12 15.11 For thermoplastic polymers, cite five factors that favor brittle fracture. For thermoplastic polymers, five factors that favor brittle fracture are as follows: (1) a reduction in temperature, (2) an increase in strain rate, (3) the presence of a sharp notch, (4) increased specimen thickness, and (5) modifications of the polymer structure

13 15.13 In your own words, describe the mechanisms by which semicrystalline polymers (a) elastically deform and (b) plastically deform, and (c) by which elastomers elastically deform. (a) and (b) The mechanisms by which semicrystalline polymers elastically and plastically deform are described in Section (c) The explanation of the mechanism by which elastomers elastically deform is provided in Section 15.9

14 15.14 Briefly explain how each of the following influences the tensile modulus of a semicrystalline polymer and why: (a) Molecular weight (b) Degree of crystallinity (c) Deformation by drawing (d) Annealing of an undeformed material (f) Annealing of a drawn material (a) The tensile modulus is not directly influenced by a polymer's molecular weight. (b) Tensile modulus increases with increasing degree of crystallinity for semicrystalline polymers. This is due to enhanced secondary interchain bonding which results from adjacent aligned chain segments as percent crystallinity increases. This enhanced interchain bonding inhibits relative interchain motion. (c) Deformation by drawing also increases the tensile modulus. The reason for this is that drawing produces a highly oriented molecular structure, and a relatively high degree of interchain secondary bonding. (d) When an undeformed semicrystalline polymer is annealed below its melting temperature, the tensile modulus increases. (e) A drawn semicrystalline polymer that is annealed experiences a decrease in tensile modulus as a result of a reduction in chain-induced crystallinity, and a reduction in interchain bonding forces.

15 15.15 Briefly explain how each of the following influences the tensile or yield strength of a semicrystalline polymer and why: (a) Molecular weight (b) Degree of crystallinity (c) Deformation by drawing (d) Annealing of an undeformed material (a) The tensile strength of a semicrystalline polymer increases with increasing molecular weight. This effect is explained by increased chain entanglements at higher molecular weights. (b) Increasing the degree of crystallinity of a semicrystalline polymer leads to an enhancement of the tensile strength. Again, this is due to enhanced interchain bonding and forces; in response to applied stresses, interchain motions are thus inhibited. (c) Deformation by drawing increases the tensile strength of a semicrystalline polymer. This effect is due to the highly oriented chain structure that is produced by drawing, which gives rise to higher interchain secondary bonding forces. (d) Annealing an undeformed semicrystalline polymer produces an increase in its tensile strength.

16 15.21 Would you expect the tensile strength of polychlorotrifluoroethylene to be greater than, the same as, or less than that of a polytetrafluoroethylene specimen having the same molecular weight and degree of crystallinity? Why? The strength of a polychlorotrifluoroethylene having the repeat unit structure will be greater than for a polytetrafluoroethylene having the same molecular weight and degree of crystallinity. The replacement of one fluorine atom within the PTFE repeat unit with a chlorine atom leads to a higher interchain attraction, and, thus, a stronger polymer. Furthermore, poly(vinyl chloride) is stronger than polyethylene (Table 15.1) for the same reason For each of the following pairs of polymers, plot and label schematic stress strain curves on the same graph [i.e., make separate plots for parts (a), (b), and (c)]. (a) Isotactic and linear polypropylene having a weight-average molecular weight of 120,000 g/mol; atactic and linear polypropylene having a weight-average molecular weight of 100,000 g/mol (b) Branched poly(vinyl chloride) having a degree of polymerization of 2000; heavily crosslinked poly(vinyl chloride) having a degree of polymerization of 2000 (c) Poly(styrene-butadiene) random copolymer having a number-average molecular weight of 100,000 g/mol and 10% of the available sites crosslinked and tested at 20 C; poly(styrene-butadiene) random copolymer having a number-average molecular weight of 120,000 g/mol and 15% of the available sites crosslinked and tested at -85 C. Hint: poly(styrene-butadiene) copolymers may exhibit elastomeric behavior. (a) Shown below are the stress-strain curves for the two polypropylene materials. These materials will display the stress-strain behavior of a normal plastic, curve B in Figure However, the isotactic/linear will have a higher degree of crystallinity (since isotactic are more likely to crystallize than atactic/linear), and therefore, will have a higher tensile modulus and strength. Furthermore, the isotactic/linear also has a higher molecular weight which also leads to an increase in strength.

17 (b) Shown below are the stress-strain curves for the two polyvinyl chloride materials. The branched PVC will probably display the stress-strain behavior of a plastic, curve B in Figure However, the heavily crosslinked PVC will undoubtedly have a higher tensile modulus, and, also a higher strength, and will most likely fail in a brittle manner--as curve A, Figure 15.1; these are the typical characteristics of a heavily crosslinked polymer. (c) Shown below are the stress-strain curves for the two poly(styrene-butadiene) random copolymers. The copolymer tested at 20 C will display elastomeric behavior (curve C of Figure 15.1) inasmuch as it is a random copolymer that is lightly crosslinked; furthermore, the temperature of testing is above its glass transition temperature. On the other hand, since -85 C is below the glass transition temperature of the poly(styrene-butadiene) copolymer, the stress-strain behavior under these conditions is as curve A of Figure 15.1.

18

19

### Hydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules

14-1 CHAPTER 14 POLYMER STRUCTURES PROBLEM SOLUTIONS Hydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules 14.1 The repeat unit structures called for are sketched below. (a Polychlorotrifluoroethylene

### Hydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules

14-1 CHAPTER 14 POLYMER STRUCTURES PROBLEM SOLUTIONS Hydrocarbon Molecules Polymer Molecules The Chemistry of Polymer Molecules 14.1 The repeat unit structures called for are sketched below. (a Polychlorotrifluoroethylene

### (10 4 mm -2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi

CHAPTER 8 DEFORMATION AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 8.1 To provide some perspective on the dimensions of atomic defects,

### HW 10. = 3.3 GPa (483,000 psi)

HW 10 Problem 15.1 Elastic modulus and tensile strength of poly(methyl methacrylate) at room temperature [20 C (68 F)]. Compare these with the corresponding values in Table 15.1. Figure 15.3 is accurate;

### Stress Strain Behavior (I) Stress Strain Behavior (II) Stress Strain Behavior (III)

Chapter Outline: Characteristics, Applications, and Processing of Polymers Mechanical properties Stress-Strain Behavior Deformation of Semicrystalline Polymers Crystallization, Melting, Glass Transition

### 15.32 Of those polymers listed in Table 15.2, which polymer(s) would be best suited for use as ice cube trays? Why?

15.31 Name the following polymer(s) that would be suitable for the fabrication of cups to contain hot coffee: polyethylene, polypropylene, poly(vinyl chloride), PET polyester, and polycarbonate. Why? This

### Polymers: Introduction

Chapter Outline: Polymer Structures Hydrocarbon and Polymer Molecules Chemistry of Polymer Molecules Molecular Weight and Shape Molecular Structure and Configurations Copolymers Polymer Crystals Optional

### Lecture 4.1: Thermoplastics and Thermosets

Lecture 4.1: Thermoplastics and Thermosets The word plastic comes from the Greek word Plastikos, meaning able to be shaped and molded. Plastics can be broadly classified into two major groups on the basis

### MAE 20 Winter 2011 Assignment 5

MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the

### Polymer contains repeating units. A polymer is a macromolecule...but a macromolecule may not be a polymer

Polymer contains repeating units Macromolecules contain no repeating units, examples are DNA, proteins, etc A polymer is a macromolecule...but a macromolecule may not be a polymer Many + Parts The repeating

### Properties of Matter

Mr. Patrick J Camilleri B.Ed (Hons) M.Ed Science (Sheffield) Department of Physics JC Malta Properties of Matter Basics You Should Know Elasticity. Young modulus 1. Hooke's law. Extension α tension (force

### Question 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm

14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.

### Engr Materials Science and Engineering TEST 4 -- Sample Solution

Engr 70 -- Materials Science and Engineering TEST 4 -- Sample Solution Part : Solve each of the following problems completely. 1. In this problem we are asked to show that the minimum cation-to-anion radius

### CONCEPT CHECK QUESTIONS AND ANSWERS. Chapter 2 Atomic Structure and Interatomic Bonding

CONCEPT CHECK QUESTIONS AND ANSWERS Chapter 2 Atomic Structure and Interatomic Bonding Concept Check 2.1 Question: Why are the atomic weights of the elements generally not integers? Cite two reasons. Answer:

### Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras

Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module - 2 Lecture - 3 Structure of Solids This is the third part of the lecture

### Tensile Testing of Steel

C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0 - INTRODUCTION See General Lab Report Format

### CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS

CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a free-body diagram),

### Polymer Chemistry. 3.1 What is a Polymer?

3 asic Polymer hemistry Polymer chemistry is a very complex subject. The basic information presented here is sufficient for the reader to gain a good understanding of polymers which forms the base for

### Unit 2: Science for Engineering LO4: Understand properties of materials - Force-extension graphs Instructions and answers for teachers

Unit 2: Science for Engineering LO4: Understand properties of materials - Force-extension graphs Instructions and answers for teachers These instructions should accompany the OCR resource Force-extension

### Tensile Testing. Objectives

Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able

### , to obtain a way to calculate stress from the energy function U(r).

BIOEN 36 013 LECTURE : MOLECULAR BASIS OF ELASTICITY Estimating Young s Modulus from Bond Energies and Structures First we consider solids, which include mostly nonbiological materials, such as metals,

### Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied

Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the

### Solution for Homework #1

Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen

### Chapter Outline. Mechanical Properties of Metals How do metals respond to external loads?

Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility

### Objectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.

Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity

### Tensile Testing Laboratory

Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental

### AMPLITUDE AND FORCE PROFILING: STUDIES IN ULTRASONIC WELDING OF THERMOPLASTICS

AMPLITUDE AND FORCE PROFILING: STUDIES IN ULTRASONIC WELDING OF THERMOPLASTICS David A. Grewell Branson Ultrasonics Corporation ABSTRACT This paper reviews effects of amplitude and force control during

### CHARACTERIZATION OF POLYMERS BY TMA. W.J. Sichina, National Marketing Manager

PERKIN ELMER Polymers technical note CHARACTERIZATION OF POLYMERS BY W.J. Sichina, National Marketing Manager Thermomechanical analysis () is one of the important characterization techniques in the field

### Dielectric Analysis Permittivity and dielectric loss 100. Dynamic Mechanical Analysis Mechanical strength and energy loss 200

Relative Signal Technique Property Measured Change at Tg Differential Scanning Calorimetry Heat flow (heat capacity) 0.2 Thermomechanical Analysis Expansion coefficient or softening 3 Dielectric Analysis

### T and Strain Rate: Thermoplastics 0 0 0.1 0.2 0.3 4 C 20 C 40 C

T and Strain Rate: Thermoplastics Decreasing T... --increases E --increases TS --decreases %EL Increasing strain rate... --same effects as decreasing T. σ(mpa) 80 60 40 4 C 20 C 40 C Data for the semicrystalline

### Thermoplastic composites

Thermoplastic composites Definition By definition, a thermoplastic is a material based on polymer (macromolecular compound) which can be shaped, in a liquid (viscous) state at a temperature either higher

### MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions

MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,

### Polymer Melt Rheology. Introduction to Viscoelastic Behavior. Time-Temperature Equivalence

Topics to be Covered Polymer Melt Rheology Introduction to Viscoelastic Behavior Time-Temperature Equivalence Chapter 11 in CD (Polymer Science and Engineering) Polymer Melt Rheology δ τ xy Newton s Law

### Effect of Sterilization Techniques on Polymers

Effect of Sterilization Techniques on Polymers Contents of Presentation Introduction to Polymers Properties and Stability of Polymers Affect of Ionising Radiation and Ethylene Oxide on Polymers The need

### σ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?

Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials

### TENSILE TESTING PRACTICAL

TENSILE TESTING PRACTICAL MTK 2B- Science Of Materials Ts epo Mputsoe 215024596 Summary Material have different properties all varying form mechanical to chemical properties. Taking special interest in

### CHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS

19-1 CHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS Heat Capacity 19.1 The energy, E, required to raise the temperature of a given mass of material, m, is the product of the specific heat, the mass of

### (10 4 mm -2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi

14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide

### The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R

3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated

### Low Temperature Properties of Polymers

TECHNICAL WHITEPAPER Low Temperature Properties of Polymers Introduction Most plastics at room temperature show their familiar properties of flexibility (a low Young s modulus) and high resistance to cracking

### TENSILE AND CREEP DATA OF 316L (N) STAINLESS STEEL ANALYSIS

TENSILE AND CREEP DATA OF 316L (N) STAINLESS STEEL ANALYSIS V. Bindu Neeharika, K. S. Narayana, V. Krishna and M. Prasanth Kumar Mechanical Department, ANITS, Sangivalasa, Visakhapatnam India binduneeharika@yahoo.co.in

### Concepts of Stress and Strain

CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original

### Plastic Behaviour - Tensile Strength

Plastic Behaviour - Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hot-rolled, cold-rolled, heat treated, etc.).

### The mechanical properties of metal affected by heat treatment are:

Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.

### A8 Thermal properties of materials

A8 Thermal properties of materials Thermal properties the melting temperature, T m, and the glass temperature (temperatura de transição vítrea), T g, relate directly to the strength of the bonds in the

### Long term performance of polymers

1.0 Introduction Long term performance of polymers Polymer materials exhibit time dependent behavior. The stress and strain induced when a load is applied are a function of time. In the most general form

### Fatigue Testing. Objectives

Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students

### CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS

7-1 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length

### Developments in Low Temperature Testing of Rubber Materials

Developments in Low Temperature Testing of Rubber Materials Technical report 01/4, 2nd edition Nov 2010 Göran Spetz Elastocon AB SWEDEN Introduction The low temperature properties of rubber materials are

### LABORATORY EXPERIMENTS TESTING OF MATERIALS

LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective

### Developing an ANSYS Creep Model for Polypropylene from Experimental Data

Developing an ANSYS Creep Model for Polypropylene from Experimental Data Abstract Martin J. Dropik David H. Johnson, P.E. David E. Roth, P.E. Penn State-Erie, Erie, PA, USA This paper describes a procedure

### Chapter Outline Dislocations and Strengthening Mechanisms

Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip

### Notes on Polymer Rheology Outline

1 Why is rheology important? Examples of its importance Summary of important variables Description of the flow equations Flow regimes - laminar vs. turbulent - Reynolds number - definition of viscosity

### 17 / Thermal Properties

Chapter 17 / Thermal Properties This photograph shows a white-hot cube of a silica fiber insulation material, which, only seconds after having been removed from a hot furnace, can be held by its edges

### Objective To conduct Charpy V-notch impact test and determine the ductile-brittle transition temperature of steels.

IMPACT TESTING Objective To conduct Charpy V-notch impact test and determine the ductile-brittle transition temperature of steels. Equipment Coolants Standard Charpy V-Notched Test specimens Impact tester

### Composition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)

10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature

### PROPERTIES OF MATERIALS

1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties

### METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING

METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B-306) INTRODUCTION TENSION TEST Mechanical testing

### In order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 10-3 m. Thus,

5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,

### Introduction to Aerospace Engineering

Introduction to Aerospace Engineering Lecture slides Challenge the future 1 Material types Metals, polymers, ceramics, composites Faculty of Aerospace Engineering 6-12-2011 Delft University of Technology

### STRESS-STRAIN CURVES

STRESS-STRAIN CURVES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 August 23, 2001 Introduction Stress-strain curves are an extremely

### Chapter Outline Dislocations and Strengthening Mechanisms

Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip

### Elements of Addition Polymerization. Branching and Tacticity. The Effect of Crystallinity on Properties

Topics to be Covered Elements of Addition Polymerization Branching and Tacticity The Effect of Crystallinity on Properties Chapters 1 & 2 in CD (Polymer Science and Engineering) What Are Polyolefins? The

### TIE-31: Mechanical and thermal properties of optical glass

PAGE 1/10 1 Density The density of optical glass varies from 239 for N-BK10 to 603 for SF66 In most cases glasses with higher densities also have higher refractive indices (eg SF type glasses) The density

### PLASTIC DEFORMATION AND STRESS-STRAIN CURVES

PLASTIC DEFORMATION AND STRESS-STRAIN CURVES Introduction Background Unit: Plastic Deformation and Stress-Strain Curves In the last unit we studied the elastic response of materials to externally applied

### Chapter Outline. Mechanical Properties of Metals How do metals respond to external loads?

Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility

### KMχ /γ = (1.3E -23 )(88.2)(3.4138 E 20 ) 3.05 = 0.12834. T g = (302)*( 0.12834 / (1-0.12834) ) = 44.5 o K

Problem Set #5 Solutions Chemical ngineering 60/60 Problem 8.4 We re given T g as 0 o C and given the viscosity at 5 o C, and asked to find the viscosity at 40 o C. We can use equation 8.48 (WLF equation).

### Material Science. Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore India

Material Science Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore 5612 India Chapter 15. Thermal properties Engineering materials are important

### THE IMPACT OF YIELD STRENGTH OF THE INTERCONNECTOR ON THE INTERNAL STRESS OF THE SOLAR CELL WITHIN A MODULE

5th World Conference on Photovoltaic Energy Conversion, 6-1 September 21, Valencia, Spain THE IMPACT OF YIELD STRENGTH OF THE INTERCONNECTOR ON THE INTERNAL STRESS OF THE SOLAR CELL WITHIN A MODULE Y.

### Why Plastic Products Fail

A Smithers Group Company 0 Why Plastic Products Fail Jenny Cooper Commercial Manager Dr Chris O Connor - Director of Consultancy Smithers Rapra 1 To provide our customers with Research, Consultancy and

### Torsion Testing. Objectives

Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials

### MAL 201E: Materials Science. COURSE MATERIALS (with text) GRADING 25.09.2012 COURSE SCHEDULE

MAL 201E: Materials Science Course Objective... Introduce fundamental concepts in Materials Science You will learn about: material structure how structure dictates properties how processing can change

### STRAIN-LIFE (e -N) APPROACH

CYCLIC DEFORMATION & STRAIN-LIFE (e -N) APPROACH MONOTONIC TENSION TEST AND STRESS-STRAIN BEHAVIOR STRAIN-CONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESS-STRAIN BEHAVIOR STRAIN-BASED APPROACH TO

### Material Strengthening Mechanisms. Academic Resource Center

Material Strengthening Mechanisms Academic Resource Center Agenda Definition of strengthening Strengthening mechanisms Grain size reduction Solid solution alloying Cold Working (strain hardening) Three

### 3 rd Year Dental Materials Science

3 rd Year Dental Materials Science Dr. Graham Cross School of Physics and CRANN SFI Nanoscience Building, Rm 1.5 http://www.tcd.ie/physics/people/graham.cross/ Graham.Cross@tcd.ie 16.11.2007 Dental Materials

### Distinguishing strength from toughness. Understanding fracture toughness.

Lecture notes version 20 Oct 2010 Chapter 8 Fracture and fracture toughness A fractured Liberty Ship 8.1 Introduction and synopsis Distinguishing strength from toughness. Understanding fracture toughness.

### 3. Test Methods for Evaluation of ESCR of Plastics

3. Test Methods for Evaluation of ESCR of Plastics A common laboratory request for ESC-prone polymers is to check ESCR performance for quality control, competitive product evaluations, and research and

### Mechanics of Materials-Steel

Mechanics of Materials-Steel Structural Steel Structural steel considered one of the predominant materials for construction of buildings, bridges, towers and other structures. The preferable physical properties

### Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras

Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module - 2 Lecture - 2 Part 2 of 2 Review of Atomic Bonding II We will continue

### Environmental Stress Crack Resistance of Polyethylene Pipe Materials

Environmental Stress Crack Resistance of Polyethylene Pipe Materials ROBERT B. TAMPA, Product Development and Service Engineer* Abstract Slow crack growth is a phenomenon that can occur in most plastics.

### Measurement of Residual Stress in Plastics

Measurement of Residual Stress in Plastics An evaluation has been made of the effectiveness of the chemical probe and hole drilling techniques to measure the residual stresses present in thermoplastic

### UROP- Annealed 3D printed parts- Final Write up Michael Rosplock Abstract

UROP- Annealed 3D printed parts- Final Write up Michael Rosplock Abstract The purpose of this study was to examine the effects of a basic annealing process on 3D printed tensile test samples. Several different

### Environmental Stress Crack Resistance Of Polyethylene

Introduction to Environmental Stress Cracking and ESCR Over the past decade, high-density polyethylene (HDPE) materials have improved significantly and now meet more stringent performance standards; some

### Griffith theory of brittle fracture:

Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials

### PROCESSING OF VARIOUS MATERIALS

4 PROCESSING OF VARIOUS MATERIALS CHAPTER CONTENTS 4.1 Shaping Processes for Polymers Polymers Manufacturing Processes for Polymers 4.2 Rubber Processing Technology Processing of rubber into finished good

### 14:635:407:02 Homework III Solutions

14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.

### Materials Issues in Fatigue and Fracture

Materials Issues in Fatigue and Fracture 5.1 Fundamental Concepts 5.2 Ensuring Infinite Life 5.3 Finite Life 5.4 Summary FCP 1 5.1 Fundamental Concepts Structural metals Process of fatigue A simple view

### σ y ( ε f, σ f ) ( ε f

Typical stress-strain curves for mild steel and aluminum alloy from tensile tests L L( 1 + ε) A = --- A u u 0 1 E l mild steel fracture u ( ε f, f ) ( ε f, f ) ε 0 ε 0.2 = 0.002 aluminum alloy fracture

### Solution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.

14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius

### Resistance of Plastics to Gamma Irradiation

Elastomers 1 MATERIAL TOLERANCE LEVEL (kgy) COMMENTS Butyl 50 Sheds particulate after irradiation. Ethylene Propylene 100 200 Crosslinks, yellows slightly. Diene Monomer (EPDM) Fluoro Elastomer 50 Avoid

### Thermoplastic Material Testing for Use in Sigmasoft

Thermoplastic Material Testing for Use in Sigmasoft + technical center for materials a DatapointLabs affiliate Materials Testing Data Infrastructure Productivity Software Plastic Rubber Film Metal Foam

### Stress Strain Relationships

Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the

### Stress. tensile. elongation at yield. yield stress. weight. elascity modulus. strain velocity 13%/min

3 Mechanical Properties 3 1 Tensile Strength The -strain curve when tension is applied to ASTM-D638 type 1 test piece of Iupilon / NOVAREX at a strain velocity of 5mm/min is shown in Fig. 3 1 1. The following

### Uniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng

Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics

### Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3

Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which

### Guide to the measurement of the flow properties of polymeric materials

Guide to the measurement of the flow properties of polymeric materials In processing plastics the material is melted, transferred and then solidified. The transfer or flow process is critical to processing

Evaluation on Wire Covering Degradation (Investigation of ADEOS-II Malfunction) Electronic, Mechanical Components and Materials Engineering Group Institute of Aerospace Technology Japan Aerospace Exploration

### FTIR and DSC of polymer films used for packaging: LLDPE, PP and PVDC

FTIR and DS of polymer films used for packaging: LLDPE, PP and PVD John Petrovich SHAPE American High School Abstract: Polymers are compounds used in various materials. There are a plethora of methods